long lived radioisotope has a half life of "only" around a year, there are often proposals to recover ruthenium in a new kind of nuclear reprocessing from spent fuel. An unusual ruthenium deposit can also be found at the natural nuclear fission reactor that was active in Oklo, Gabon some two billion years ago. Indeed, the isotope ratio of ruthenium found there was one of several ways used to confirm that a nuclear fission chain reaction had indeed occurred at that site in the geological past. Uranium is no longer mined at Oklo and there have never been serious attempts to recover any of the platinum group metals present there. Production Roughly 30 tonnes of ruthenium are mined each year with world reserves estimated at 5,000 tonnes. The composition of the mined platinum group metal (PGM) mixtures varies widely, depending on the geochemical formation. For example, the PGMs mined in South Africa contain on average 11% ruthenium while the PGMs mined in the former USSR contain only 2% (1992). Ruthenium, osmium, and iridium are considered the minor platinum group metals. Ruthenium, like the other platinum group metals, is obtained commercially as a by-product from nickel, and copper, and platinum metals ore processing. During electrorefining of copper and nickel, noble metals such as silver, gold, and the platinum group metals precipitate as anode mud, the feedstock for the extraction. The metals are converted to ionized solutes by any of several methods, depending on the composition of the feedstock. One representative method is fusion with sodium peroxide followed by dissolution in aqua regia, and solution in a mixture of chlorine with hydrochloric acid. Osmium, ruthenium, rhodium, and iridium are insoluble in aqua regia and readily precipitate, leaving the other metals in solution. Rhodium is separated from the residue by treatment with molten sodium bisulfate. The insoluble residue, containing Ru, Os, and Ir is treated with sodium oxide, in which Ir is insoluble, producing dissolved Ru and Os salts. After oxidation to the volatile oxides, is separated from by precipitation of (NH4)3RuCl6 with ammonium chloride or by distillation or extraction with organic solvents of the volatile osmium tetroxide. Hydrogen is used to reduce ammonium ruthenium chloride yielding a powder. The product is reduced using hydrogen, yielding the metal as a powder or sponge metal that can be treated with powder metallurgy techniques or argon-arc welding. Ruthenium is contained in spent nuclear fuel both